Review: current international research into cellulose nanoﬁbres
S. J. EichhornÆA. Dufresne ÆM. ArangurenÆ N. E. MarcovichÆ
J. R. CapadonaÆS. J. RowanÆC. WederÆW. ThielemansÆM. Roman Æ S. RenneckarÆ W. GindlÆS. VeigelÆ J. KeckesÆH. YanoÆ K. AbeÆ M. NogiÆ A. N. NakagaitoÆ A. MangalamÆJ. SimonsenÆA. S. Benight Æ A. BismarckÆL. A. BerglundÆT. Peijs
Abstract This paper provides an overview of recent progress made in the area of cellulose nanoﬁbre-based nanocomposites. An introduction into the methods used to isolate cellulose nanoﬁbres (nanowhiskers, nanoﬁbrils) is given, with details of their structure. Following this, the article is split into sections dealing with processing and characterisation of cellulose nanocomposites and new developments in the area, with particular emphasis on applications. The types of cellulose nanoﬁbres covered are those extracted from plants by acid hydrolysis
(nanowhiskers), mechanical treatment and those that occur naturally (tunicate nanowhiskers) or under culturing con-ditions (bacterial cellulose nanoﬁbrils). Research high-lighted in the article are the use of cellulose nanowhiskers for shape memory nanocomposites, analysis of the inter-facial properties of cellulose nanowhisker and nanoﬁbril-based composites using Raman spectroscopy, switchable interfaces that mimic sea cucumbers, polymerisation from the surface of cellulose nanowhiskers by atom transfer radical polymerisation and ring opening polymerisation,
S. J. Eichhorn (&)
Materials Science Centre, School of Materials and the Northwest Composites Centre, Grosvenor Street, Manchester M1 7HS, UK e-mail: firstname.lastname@example.org
Grenoble Institute of Technology, The International School of Paper, Print Media & Biomaterials (Grenoble INP Pagora), BP65, 38402 Saint Martin D’He`res Cedex, France
M. ArangurenN. E. Marcovich
National Institute of Research in Science and Technology of Materials (INTEMA), Universidad Nacional de Mar del Plata, Av. Juan B. Justo 4302, B7608FDQ Mar del Plata, Argentina J. R. Capadona
Rehabilitation Research and Development, Louis Stokes Cleveland DVA Medical Center, 10701 East Blvd., Cleveland, OH 44106, USA
S. J. Rowan
Department of Macromolecular Science and Engineering, Case Western Reserve University (CWRU), 2100 Adelbert Road, Cleveland, OH 44106, USA
Adolphe Merkle Institute, University of Fribourg, 1700 Fribourg, Switzerland
School of Chemistry and Process and Environmental Research Division, Faculty of Engineering, The University of Nottingham, Nottingham NG7 2RD, UK
M. RomanS. Renneckar
Department of Wood Science and Forest Products, Virginia Tech, 230 Cheatham Hall, 0323, Blacksburg, VA 24061, USA W. Gindl
Department of Materials Science and Process Engineering, University of Natural Resources and Applied Life Sciences, BOKU-Vienna, Austria
Wood K plus, Competence Centre for Wood Composites and Wood Chemistry, Linz, Austria
Department of Materials Physics, Erich Schmid Institute of Materials Science, Austrian Academy of Sciences, University of Leoben, Leoben, Austria
H. YanoK. AbeM. NogiA. N. Nakagaito
Research Institute for Sustainable Humanosphere, Kyoto University, Uji, Kyoto 611-0011, Japan
Published in "Journal of Materials Science 45(1): 1-33, 2010" which should be cited to refer to this work.
and methods to analyse the dispersion of nanowhiskers. The applications and new advances covered in this review are the use of cellulose nanoﬁbres to reinforce adhesives, to make optically transparent paper for electronic displays, to create DNA-hybrid materials, to generate hierarchical composites and for use in foams, aerogels and starch nanocomposites and the use of all-cellulose nanocompos-ites for enhanced coupling between matrix and ﬁbre. A comprehensive coverage of the literature is given and some suggestions on where the ﬁeld is likely to advance in the future are discussed.
Introduction to cellulose structure/property relationships
Cellulose is probably one of the most ubiquitous and abundant polymers on the planet, given its widespread industrial use in the present age, but also in the past for ropes, sails, paper, timber for housing and many other applications. By far the most commercially exploited nat-ural resource containing cellulose is wood. The word ‘material’ in fact derives from the Latin for ‘trunk of tree’. Indeed, Chaucer writes in the ‘Parson’s Tale’ in 1390
‘‘For he that is in helle hath defaute of light material. for certes, the derke light that shal
Come out of the fyr that evere shal brenne’’
showing quite clearly that the relationship between wood and material was persisting into the Middle Ages.
Other plants also contain a large amount of cellulose, including hemp, ﬂax, jute, ramie and cotton. In addition to these, there are non-plant sources of cellulose; for instance, forms produced by bacteria and cellulose produced by tunicates. Bacterial cellulose (BC) is produced by the gram-negative bacteria Acetobacter xylinum (or Gluconacetob-acter xylinum), which manifests itself under special cultur-ing conditions as a ﬁne ﬁbrous network of ﬁbres . Tunicate cellulose is produced by sea creatures (e.g. Microcosmus fulcatus) in the form of rod-like near perfect crystals of the material .
Since cellulose is classed as a carbohydrate (a sub-stance containing carbon, hydrogen and oxygen), it is necessary to point out that although this term applies to a large number of organic compounds, cellulose is unique in that it can be either synthesised from, or hydrolysed to, monosaccharides . The repeat unit of the cellulose polymer is known to comprise two anhy-droglucose rings joined via a b-1,4 glycosidic linkage from this unit  (called cellobiose) as shown in Fig.1. In its native form cellulose is typically called cellulose-I. This cellulose-I crystal form, or native cellulose, also comprises two allomorphs, namely cellulose Ia and Ib . The ratio of these allomorphs is found to vary from plant species to species, but bacterial and tunicate forms are Ia and Ib rich, respectively [6, 7]. The crystal structures of cellulose allomorphs Ia and Ib have been determined with great accuracy, particularly the complex hydrogen bonding system [6, 7]. The hydrogen bond network makes cellulose a relatively stable polymer, which does not readily dissolve in typical aqueous sol-vents and has no melting point. This network also gives the cellulose chains a high axial stiffness . Since high stiffness is a desirable property for a reinforcement ﬁbre in a composite, the determination of the crystal modulus of cellulose will be reviewed later.
Cellulose chains aggregate into the repeated crystal-line structure to form microﬁbrils in the plant cell wall, which also aggregate into larger macroscopic ﬁbres. It is this hierarchical structure that is essentially deconstructed in order to generate cellulose nanoﬁbres from plants. BC and whiskers produced by tunicates already exist in
Department of Wood Science and Forest Products,
Virginia Tech, 248 Cheatham Hall, Blacksburg, VA 24061, USA J. Simonsen
Department of Wood Science & Engineering, Oregon State University, Corvallis, OR 97331, USA
A. S. Benight
Departments of Chemistry & Physics, Portland State University, Portland, OR, USA
Department of Chemical Engineering, Polymer and Composite Engineering Group (PACE), Imperial College London, London, UK
L. A. Berglund
Department of Fibre & Polymer Technology, Wallenberg Wood Science Centre, KTH, 10044 Stockholm, Sweden
Centre for Materials Research, Queen Mary, University of London, Mile End Road, London E1 4NS, UK
O O OH O OH OH O H O HO OH n
Fig. 1 The repeat unit of cellulose
this form, making them desirable materials for niche applications.
The study of cellulosic nanoﬁbres as a reinforcing phase in nanocomposites started 15 years ago . Since then a huge amount of literature has been devoted to cellulose nanoﬁbres, and it is becoming an increasingly topical subject. Different descriptors of these nanoﬁbres are often referred to in the literature. These include ‘‘nanowhiskers’’ (or just simply ‘‘whiskers’’), ‘‘nanocrystals’’ or even ‘‘monocrystals’’. These crystallites have also often been referred to in literature as ‘‘microﬁbrils’’, ‘‘microcrystals’’ or ‘‘microcrystallites’’, despite their nanoscale dimensions. The term ‘‘whiskers’’ is used to designate elongated crys-talline rod-like nanoparticles, whereas the designation ‘‘nanoﬁbrils’’ should be used to designate long ﬂexible nanoparticles consisting of alternating crystalline and amorphous strings.1
In essence, the principle reason to utilise cellulose nanoﬁbres in composite materials is because one can potentially exploit the high stiffness of the cellulose crystal for reinforcement. This can be done by breaking down the hierarchical structure of the plant into individ-ualised nanoﬁbres of high crystallinity, therefore reducing the amount of amorphous material present. Since plant ﬁbres are hierarchically ﬁbrous it is possible to do this, yielding a ﬁbrous form of the material (nanowhiskers, nanoﬁbrils), which due to their aspect ratio (length/ diameter) and therefore reinforcing capabilities are potentially suitable for composite materials. A high aspect ratio to the ﬁbres is desirable as this enables a critical length for stress transfer from the matrix to the rein-forcing phase. This will be discussed in more detail once the mechanical properties of cellulose nanoﬁbres have been presented.
It is however not clear what the true crystal modulus of cellulose is, nor whether this stiffness is really obtainable from plants, bacteria or tunicates. Establishing a true value of the crystal modulus of cellulose sets an upper limit to what is achievable in terms of reinforcing potential.
The crystal modulus of cellulose was ﬁrst determined in 1936 by Meyer and Lotmar  using a theoretical model and bond stiffness constants derived from spec-troscopic measurements. They obtained a value of*120 GPa, which is close to values that were later
experimentally conﬁrmed for this property [10, 11]. Despite this prediction, Meyer and Lotmar used an incorrect structure for cellulose, and so when this was corrected by Lyons, and a value of 180 GPa was obtained . Lyons however used an incorrect term in his mathematical expression for bond angle bending. This was rectiﬁed by Treloar , who reported a modulus of 56 GPa. This value is now considered to be too low, probably due to the lack of intramolecular hydrogen bonding in Treloar’s cellulose structure . Sakurada et al.  reported a value of 138 GPa for the crystal modulus of cellulose, which was determined using X-ray diffraction of deformed ﬁbre bundles. This paved the way for many more measurements and determinations of the crystal modulus of cellulose using X-ray diffraction [11, 14] and theoretical approaches [15–18], all of which have obtained values in the range 100–160 GPa. A more recent determination of the cellulose crystal modulus using inelastic X-ray scattering (IXS) reported a value of 220 GPa . Such a high crystal modulus for cellulose has not been reported before, but this may be due to the fact that the assumption of uniform stress in the crystals of cellulose, a basic assumption for most crystal modulus determinations, is not correct [19,20]. This high value for the crystal modulus does however call into question the-oretical approaches, and since they are consistent with experiment it may be that a more modest value is appropriate. Nevertheless, this value of the modulus of crystalline cellulose is quite large compared to other materials, especially if its comparatively lower density is taken into account. The moduli of a number of commonly used engineering materials are reported in Table 1. Also reported are the speciﬁc moduli (modulus/density), which show that the speciﬁc modulus of crystalline cellulose exceeds engineering materials such as steel, concrete, glass and aluminium. It is worth pointing out that cellu-lose has obvious disadvantages compared to traditional engineering materials; for instance, moisture absorption and swelling, and enzymatic degradability to name but two. It is worth pointing out that the microﬁbrils com-prising plants do not swell themselves, as it is not ener-getically favourable for water to penetrate the bulk material.
1 For the sake of clarity and consistency the term ‘‘nanowhiskers’’
will be used to describe material hydrolysed from plants, and ‘‘nanoﬁbrils’’ for material extracted by mechanical means or from native sources such as bacterial cellulose. The term ‘‘nanoﬁbres’’ will be used as a general descriptor of both these sub-forms of reinforcement.
Table 1 Moduli of engineering materials compared to cellulose
Material Modulus (GPa) Density (Mg m-3) Speciﬁc modulus (GPa Mg-1m3) Reference Aluminium 69 2.7 26  Steel 200 7.8 26  Glass 69 2.5 28  Crystalline cellulose 138 1.5 92 
The crystalline modulus of cellulose is hard to achieve in reality for a micron-sized ﬁbre. Plant ﬁbres often have moduli well below the crystalline value. Typical values of the modulus of a range of cellulose ﬁbres are given in Table2. When the density of the ﬁbres is taken into account and speciﬁc modulus is determined (assuming a density of cellulose of 1.5 Mg m-3), then the values approachthose of glass and other engineering solids. Many authors have published values for the modulus of plant ﬁbres, some closer to the crystal modulus of cellulose quoted in Table1. It is however difﬁcult to obtain an accurate modulus for plant ﬁbres, given their often irreg-ular and variable cross-sections and the presence of voids in the form of lumens. It is beyond the scope of this article to fully review this aspect of natural ﬁbre mechanics, but it is acknowledged that higher values than those quoted in Table2have been reported. Plant ﬁbres are known to have variable mechanical properties, and another reason for extracting nanoﬁbers and nanoﬁbrils from the cell wall of plants is that they are thought to have more consistent properties.
One way therefore to obtain ﬁbres that have a modulus that approaches that of pure crystalline cellulose is to break down the structure of the plant into the elementary nano-ﬁbrils, or crystals (nanowhiskers), that make up the ﬁbre. Another approach is to source material that already has these structural forms. Two examples of this latter approach are to use microbial or BC, or to take whiskers of cellulose from an animal source (such as tunicates, a sea creature). BC ﬁbrils are produced by a family of bacteria referred to as G. xylinum, under special culturing condi-tions . The ﬁbrils are generally in the form of a ﬁne non-woven mesh or network, and have been reported to have moduli in the range 78–114 GPa [22,23]. Some of the ﬁrst reports of the use of BC for composite materials appeared in the mid-1990s [24,25], but there has recently been a resurgence of this research area. Notable examples of this come from Japan at Kyoto University  and from
the UK at Imperial College [27–30], both of whom have contributed to this article.
Microﬁbrillated cellulose (MFC), where ﬁne nano-sized ﬁbrils are extracted from plants by mechanical processing and/or homogenisation, was ﬁrst reported in the early 1980s . Since then, and in more recent times, a large number of papers have been published on this topic, the full scope of which is beyond this review although an overview of the physical properties of nanoﬁbrils from this source will be given in the section ‘‘An overview of cel-lulose whisker and nanoﬁbre properties (Grenoble Institute of Technology (INPG), International School of Paper, Grenoble, France)’’. Notable recent examples of research into these materials have been by groups in Japan at Kyoto University , in Sweden at KTH , in the USA at Virginia Tech , and in Austria at BOKU, all of whom have made contributions to this article.
The existence of highly crystalline cellulose nanowhis-kers has been known for some time. They can be extracted from plant material via a controlled acid hydrolysis, which more readily hydrolyses the amorphous regions of the cellulose, leaving high aspect ratio (length to diameter ratio) crystals of pure cellulose. The ﬁrst report of cellulose crystals, produced in solution, was by Ranby and Noe in 1961 . This was followed by the ﬁrst report of the production of cellulose nanowhiskers by acid hydrolysis . Nanowhiskers of cellulose can also be extracted from the mantle of tunicates, a sea creature . Tunicate nanowhiskers are reported to have moduli of *140 GPa , but acid hydrolysed nanowhiskers are thought to have much lower moduli (50–100 GPa) . The ﬁrst report of the use of cellulose nanowhiskers in composite materials was by Favier et al. in 1995 . They investigated the percolation of nanowhiskers extracted from tunicates. Since then a large number of groups have reported on the use of cellulose nanowhiskers and their use in composites, some of whom have contributed to this article; namely from Argentina at INTEMA, within the UK at the Uni-versity of Manchester and the UniUni-versity of Nottingham, and from the USA at Case Western Reserve University, Virginia Tech and at Oregon State University.
The relative mechanical advantage of using cellulose nanoﬁbres (nanowhiskers, nanoﬁbrils) over conventional ﬁbres is best shown graphically. Figure2 shows Halpin-Tsai micromechanical predictions for unidirectional poly-propylene matrix composites ﬁlled with 50 vol% of uni-directional cellulose ﬁbres as a function of different ﬁbre aspect ratios and Young’s moduli. The Halpin-Tsai model [39,40] is a short-ﬁbre composite model which predicts all the elastic constants of composite materials as a function of the aspect ratio of the ﬁller when the constituent properties and the volume fractions of the two phases (matrix and reinforcement) are known.
Table 2 Mechanical properties of some common plant ﬁbres, namely, Young’s modulus, speciﬁc Young’s modulus, breaking strength and breaking strain
Fibre type Young’s
modulus (GPa) Speciﬁc Young’s modulus (GPa Mg-1m3) Breaking strength (GPa) Breaking strain (%) Flax 27.0 18.0 0.81 3.0 Jute 25.8 17.2 0.47 1.8 Hemp 32.6 21.7 0.71 2.2 Ramie 21.9 14.6 0.89 3.7
Data taken from Morton and Hearle  with the conversion from N
tex-1to GPa being made using a density of cellulose of 1.5 Mg m-3
The Halpin-Tsai equation can be written as Ec Em¼ 1þfguf 1guf ð1Þ with g¼ Ef Em1 Ef Emþf ð2Þ
whereEc,EfandEmare respectively the composite,
rein-forcement and matrix Young’s moduli; uf is the ﬁller
volume fraction and f a shape factor. The shape factors relative to ﬁbres reinforcement has been chosen to be (0.5s)1.8, in accordance with a previous study , wheres is the aspect ratio. For a more extensive introduction to the model, the reader is referred to the relevant scientiﬁc lit-erature [39, 40]. The model supposes a perfect interface between matrix and ﬁbre, but does not account for ﬁbre– ﬁbre interactions, which can take place in high loading cellulose composite/nanocomposites (i.e. percolated net-works). Young’s modulus of cellulose ﬁbres can vary according to the source, and ﬁbre dimensions. A modulus of 40–60 GPa is usually found for natural bast ﬁbres like ﬂax and hemp (see Table2), while it potentially increases up to 80 GPa for single cells  and certainly in the range of 100–140 GPa for nanoﬁbrils and nanowhiskers [17,23]. Due to the intrinsic higher performances of nano-sized ﬁllers, cellulose nanowhiskers are predicted to enhance stress transfer and therefore the ﬁnal composite modulus (more than 3-fold) when compared with traditional micron-sized cellulose ﬁbres. It is clear from these data why the recent interest in studying nano-cellulose composite has occurred. Nevertheless, such effects can only be realised for ﬁbres of a high-enough aspect ratio. Cellulose nanoﬁ-bres with an aspect ratio smaller than 10 would not have
any major beneﬁts when compared with conventional micron-sized ﬁlaments. Only nanoﬁbres with aspect ratios bigger than 50 can guarantee an efﬁcient reinforcement effect. For aspect ratios larger than 100, Young’s moduli reach a plateau, which correspond to the upper-limit case for reinforcement. For example, single ﬂax ﬁbres, which are around 25 mm long and 20lm thick, will have an aspect ratio of 1250, which is well above the critical value. Since cellulose nanowhiskers generally have lower aspect ratios, typically between 10 and 30, there is a need for longer nanoﬁbres of this type.
This article contains contributions to the ﬁeld of cellu-lose nanocomposites in the areas of processing and char-acterisation and applications and new advances in the subject. It is intended that a ﬂavour of current research taking place internationally will be given, rather than a general overview of the area of research. For other reviews of cellulose nanocomposites, the reader is referred to an article by Samir et al.  and another by Kamel . Before each research contribution is reported, a detailed overview of nanowhisker and nanoﬁbril properties will be given by Alain Dufresne at INP, Grenoble, France, who is a pioneer in this research area.
An overview of cellulose whisker and nanoﬁbre properties (Grenoble Institute of Technology (INPG), International School of Paper, Grenoble, France)
As already mentioned, native cellulose present in macro-scopic ﬁbres, like for instance plant ﬁbres, consists of a hierarchical structure. This hierarchical structure is built up by smaller and mechanically stronger entities consisting of native cellulose ﬁbrils. These ﬁbrils interact strongly and aggregate to form the natural or native cellulose ﬁbres. The lateral dimension of these ﬁbrils depends on the source of the cellulose but it is typically of the order of a few nanometres. The ﬁbrils contain crystalline cellulosic domains but also noncrystalline domains located at the surface and along their main axis. The noncrystalline domains form weak spots along the ﬁbril. These ﬁbrils display high stiffness and are therefore suitable for the reinforcement of nanocomposite materials.
There are numerous methods to prepare nanoﬁbres from natural cellulose ﬁbres. The properties of these nanoﬁbres will now be outlined in more detail. One method consists of submitting plant ﬁbres to strong acid conditions combined with sonication. It leads to the hydrolysis of noncrystalline domains, and rod-like nanoﬁbres called cellulose nano-whiskers result from this treatment. The dimensions of these resultant nanowhiskers depend on the source of the cellu-lose, but their length generally ranges between 100 and 300 nm. Some typical transmission electron microscope
1 10 100 1000 0 10 20 30 40 50 60 70 40 GPa 60 GPa 80 GPa 100 GPa 120 GPa E c ) a P G( Aspect ratio (L/d) φv=50 vol% 140 GPa
Fig. 2 Model plots of the Halpin-Tsai equation (Eq.1) for a range of
ﬁbre moduli showing the predicted composite modulus (Ec) as a
function of the aspect ratio of the ﬁbre reinforcement. The model assumes a unidirectional composite sample, with no ﬁbre–ﬁbre interactions and a polypropylene matrix
images of these nanowhiskers are reported in Fig.3, taken from a number of publications [45–52].
By omitting the hydrolysis step and only submitting the ﬁbres to high mechanical shearing forces, disintegra-tion of the ﬁbres occurs, leading to a material called
microﬁbrillated cellulose (MFC). A combination of high mechanical shearing forces and mild enzymatic hydrolysis can also be used to prepare MFC . These nanoﬁbrils ideally consist of individual nanoparticles with a lateral dimension around 5 nm. Generally, MFC consists of nanoﬁbril aggregates, whose lateral dimensions range between 10 and 30 nm, or more.
Among the many plant ﬁbres used for the preparation of nanowhiskers, cotton constitutes the main source. The main reason is the high cellulose content of cotton that results in a higher yield when preparing cellulose nano-whiskers and avoids intensive puriﬁcation of cellulose.
The main problem associated with making effective nanocomposites from cellulose nanoﬁbres is related to their homogeneous dispersion within a polymeric matrix. Because of the high stability of aqueous suspensions of cellulose nanowhiskers, water is the preferred processing medium. Hydrosoluble polymers are therefore well adapted for the processing of cellulose nanowhisker reinforced nanocomposites [46, 54–64]. Solid nanocomposite ﬁlms can be obtained by mixing, casting and evaporating the aqueous polymer solution and the aqueous suspension. A ﬁrst alternative consists in using an aqueous dispersed polymer, e.g. latex [50,65–75]. After mixing and casting the two aqueous suspensions, a solid nanocomposite ﬁlm can be obtained by water evaporation and particle coales-cence. A second alternative consists of using non-aqueous systems. This means that the nanoﬁbres can be dispersed in a suitable organic medium with respect to the polymeric matrix. For instance, it is possible to coat the surface of nanoﬁbres with a surfactant [45,76]. The chemical modi-ﬁcation of a nanoﬁbres’ surface is another way to obtain dispersions in organic solvents. It generally involves reactive hydroxyl groups from the surface of polysaccha-rides [77–79]. Grafting of polymeric chains to the surface of polysaccharide nanoﬁbres, using the grafting onto [80, 81] or grafting from [48, 82–84] techniques, have been reported. Recently, it was also shown that cellulose nano-whiskers can be dispersed in dimethylformamide, dimethyl sulfoxide orN-methyl pyrrolidine without additives or any surface modiﬁcations [85–87]. A solvent exchange proce-dure can also be used. Other possible processing techniques for the production of nanocomposites are ﬁltration of sus-pensions of whiskers to obtain a ﬁlm, and then immersion of this ﬁlm in a polymer solution [26,32,88–94].
Although short ﬁbres are being widely used for the processing of thermoplastic polymers and composites, very few studies have been reported concerning the processing of cellulose nanowhisker reinforced nanocomposites by melt extrusion methods . An attempt to prepare nano-composites based on cellulose nanowhiskers obtained from microcrystalline cellulose (MCC) and poly lactic acid (PLA) processed by a melt extrusion technique was
Fig. 3 Transmission electron microscope images of cellulose
whis-kers, obtained from acid hydrolysis ofa microcrystalline cellulose
,btunicate ,ccotton ,dramie ,esisal ,fstraw
,gbacterial cellulose  andhsugar beet . Reproduction of
imagesa, b, c, e and hfrom , , ,  and  with
permission from American Chemical Society (American Chemical
Society 2000, 2004, 2005, 2009); reproduction of imagedfrom 
with permission from Springer ( Springer 2008); reproduction of
image f from  with permission from Wiley ( Wiley 1996);
reproduction of imageg from  with permission from Springer
recently reported . The suspension of nanowhiskers was pumped into the polymer melt during the extrusion process. An attempt to use polyvinyl alcohol (PVA) as a compatibilizer to promote the dispersion of cellulose nanowhiskers within the PLA matrix has also been reported .
Processing and characterisation of cellulose nanocomposites
Elastomeric composites with cellulose whisker reinforcement (INTEMA, Universidad Nacional de Mar del Plata, Mar del Plata, Argentina)
Among the many applications of polyurethanes, the group at INTEMA, in collaboration with the group of Dr. Auad (Auburn University, USA), have explored the use of seg-mented polyurethanes as thermally triggered smart mate-rials. In order to separate the nanowhiskers that form the microﬁbrils entangled in the structure, the acid hydrolysis method has been utilized. The exact details of the method were based on those reported by Dong et al. .
The negative surface charge induced during the prepa-ration of cellulose nanowhiskers allows a quite stable dispersion in water [96–98]. This result initially led researchers in the area to prepare composites for which matrix and ﬁller could be dissolved/suspended in water such as latex [2, 99, 100], starch [66, 98, 101] and poly(ethylene oxide) (PEO) [57,59,60]. Further interest to extend the use of the nanowhiskers to other matrices has resulted in a study of surface modiﬁcations  and the use of surfactants  as stabilizing agents.
Mirta Aranguren and co-workers at INTEMA have expanded these options by producing a stable cellulose nanowhisker suspension in dimethylformamide to be sub-sequently incorporated in different polyurethane (PU) matrices. This approach, which had been reported previ-ously only by Dufresne’s group , involves freeze drying of the initial aqueous suspension of the nanowhiskers, and then further redispersion in DMF. Berglund and co-workers  used a slightly different approach to produce high-strength cellulose–polyurethane elastomer nanocomposites. One paramount condition for producing composites that take full advantages of the nano-size of the reinforcements is obtaining a good dispersion in the polymer. A cryogenic (liquid nitrogen) electron microscope image of cellulose nanowhiskers in polyurethane is shown in Fig.4. It is clear from this image that a good dispersion of whiskers is achieved. The dispersion of the nanowhiskers in the unreacted liquid mixture of the polyol and isocyanate was studied through the rheological characterisation of these suspensions in the linear viscoelastic range (small
deformations). Room temperature measurements on the non-catalysed system conﬁrmed that the system does not react in these conditions during the time of the test. This was also conﬁrmed by the Newtonian behaviour (constant vis-cosity) of the solution without the presence of nanowhiskers . The suspensions, on the contrary, become strongly shear-thinning by adding minimum amounts of cellulose crystals. Analysis of the storage modulus of the suspension (Fig.5) shows that a discernable change occurred with an increasing nanowhisker concentration; from a Newtonian liquid (zero storage modulus for the solution without nanowhiskers) to a viscoelastic liquid and ﬁnally to a vis-coelastic solid (cellulose nanowhisker concentrations up to 2.5 wt%). At a frequency of 1 rad s-1, a 2800-fold incre-ment in modulus of the suspension resulted from increasing the nanowhisker concentration from 0.25 to 5 wt%,
Fig. 4 A cryogenic electron microscope image of cellulose
nano-whiskers dispersed in polyurethane . Reproduction of image
from  with permission from Wiley (Wiley 2008)
10-2 10-1 100 101 102 103 10-1 100 101 102 ) a P( ' G ω (rad/s) 0 % 0.5 % 1 % 5 % 0.25% 2.5%
Fig. 5 Frequency sweep response of a mixture polyol-isocyanate and
different percentages of cellulose nanowhiskers before reaction .
Reproduction of image from  with permission from Materials
Research Society (Materials Research Society 2006)
indicative of the formation of structure in the liquid, due to a pervading network of nanowhiskers. At 5 wt% (volume fraction=0.033), a concentration that would be considered fairly low for typical ﬁllers, the low frequency viscosity is almost 6000 times that of the unﬁlled liquid mixture. A simple calculation showed that the uncured suspensions displayed a percolation behaviour with a threshold con-centration of 0.88 wt% . A polymerization reaction has also been carried out in the presence of the nanowhiskers, where their surface hydroxyl groups became covalently bonded to the matrix. The interfacial reaction was con-ﬁrmed by FTIR spectroscopy .
Among the many applications of polyurethanes, the group at INTEMA have explored the use of segmented polyurethanes as thermally triggered smart materials. These materials have the ability of ‘‘remembering’’ their original shape after being deformed and of recovering from it, as a response to an external stimulus . Because of this capability, they are also referred to as ‘‘shape mem-ory’’ polymers. This particular behaviour is the result of the two-phase molecular structure of segmented polyurethanes. One phase, called the soft segment phase, consists of a long chain diol that gives extensibility to the PU and can crys-tallize by cooling. This phase is responsible for ﬁxing a transient shape and recovering the original one. The other phase, called the hard segment phase, is formed by the isocyanate and a short diol. Extensive hydrogen bonding occurs in this phase, which can also be crystalline. Hard segments are responsible for ﬁxing the original shape. Based on the good dispersion of the cellulose nanowhiskers in a polyurethane network (as discussed previously), the INTEMA group also investigated the effect of reinforcing a shape memory PU with these nanoﬁbres. The efﬁciency of the dispersion allows the original transparency of the polymer in the composite ﬁlms produced to be maintained. Segmented polyurethanes (SPU) were synthesized to allow the introduction of the cellulose nanowhiskers before the PU reaction (SPU1), so that they became covalently attached to the polymer, and also after the reaction (SPU1*), where only physically strong interactions are possible. In both cases, the reinforcement was dispersed in DMF by ultrasonication before being used.
The sequence of incorporation of the cellulose nano-whiskers has notable consequences on the behaviour of the segmented PU . For the SPU1 experiment, the addi-tion of cellulose nanowhiskers gave typical results for the reinforcement of elastomers; an increase in modulus and a reduced elongation at break (Table3). In SPU1*, only physical interactions between the nanowhiskers and the polymer were present, which can be broken and re-built during the tensile test. The elongation at break is remark-ably less affected by the reinforcement than in the case of SPU1 (971 and 142%, respectively).
More striking was the effect of the formation of covalent bonds between the cellulose and the PU on the shape memory behaviour of the resultant ﬁlms. While the neat SPU and SPU1* showed shape memory behaviour, SPU1 did not have this capability. Cellulose covalently bonded to the matrix interferes, mainly, with the formation of the hard domains, which are responsible for ﬁxing the original shape, thus erasing the functional property of the polymer. From these results, it was clear that the cellulose nanowhiskers should be added to already synthesized PU if shape memory properties are to be maintained. Subsequent work was continued on composites prepared with a com-mercial SPU (IROGRAN PS455-203, Hunstman) and nanowhiskers. The shape memory behaviour of this system was studied through thermo-mechanical cyclic experi-ments. The samples were deformed at Ts, a temperature
above the soft segment melting temperature (Tm,s) and
below the hard segment melting temperature, so that the material exhibited rubber elasticity. After being deformed atTsand subsequently cooled belowTm,sunder constraint,
the deformed shape is ﬁxed. When reheating at Ts, the
original shape is substantially recovered due to the elastic energy stored during the deformation process.
All the nanocomposite ﬁlms displayed shape memory properties (Fig. 6), with percentages of recovery of the order of 95% (with reference to the second and subsequent cycles). Although the rigidity of the composites was markedly improved by the addition of nanowhiskers (addition of just 1 wt% of cellulose nanowhiskers increased the tensile modulus by 54% and reduced creep by 36%), extensibility of the composites was not substantially reduced. On the other hand, the improved rigidity did not have a signiﬁcant effect on the recovery of the material. The shape memory behaviour continued to be controlled by the polymer properties under the testing conditions . Interfacial micromechanics of cellulose whisker
nanocomposites (University of Manchester, Manchester, UK)
Work is underway at Manchester by Stephen Eichhorn and co-workers to investigate the reinforcing capabilities of cellulose nanowhiskers and nanoﬁbrils in composite
Table 3 Tensile properties of the SPU and nanocomposite ﬁlms: effect of cellulose incorporation sequence
Modulus (MPa) Elongation
at break (%)
SPU, 0 wt% cell 4.54±0.32 2165
SPU1, 1.0 wt% cell 6.56±1.06 142±28
SPU1*, 1.0 wt% cell 5.91±0.50 971±260
* Cellulose was incorporated after the PU had been reacted
materials, by directly measuring stresses within the nano-ﬁbres using Raman spectroscopy. This experimental approach relies on the measurement of a shift in the position of characteristic peaks within the Raman spectrum of cel-lulose when these nanocomposite materials are deformed. The materials that have been investigated so far are cellu-lose nanowhiskers produced by extraction from tunicates, acid hydrolysis of cotton and also sheets of BC. In order to deform the nanowhiskers, the group has been dispersing and embedding them in an epoxy resin beam and applying
deformation using a 4-point bending rig [17, 38]. The 4-point bending of these samples can be performed to place the whiskers in both tension and compression. Sheets of BC have been deformed in tension using a customised defor-mation rig that can be placed under the Raman spectrometer microscope.
The use of Raman spectroscopy to follow the defor-mation of polymer ﬁbres and composites began in the 1970s with the discovery that peaks within the spectrum obtained from polydiacetylene single crystals changed position with the application of tensile deformation . Following on from this, Galiotis et al. [107,108] showed that it was possible to monitor this local deformation in both single Kevlar ﬁbres, and when the same ﬁbres were embedded in a composite material. This has led to a large number of papers on a variety of composites and ﬁbre types, all of which have been recently reviewed . In recent times this technique has been used to follow the deformation mechanisms in cellulose ﬁbres and composites [110–118], and most recently cellulose nanocomposites [17,23,38].
The Raman spectrum of cellulose is dominated by a highly intense carbonyl (C–O) stretch mode, located approximately at 1095 cm-1. It is the position of this band that has been mostly used to follow the local microme-chanics of cellulose ﬁbres, although other bands such as one located at 895 cm-1, assigned to heavy atom modes (COC, COH) , have been used to follow the mechanics of cellulose ﬁbre–polymer interfaces [115,116]. The Raman band located at 1095 cm-1has been assigned to the carbonyl stretch (C–O) mode of the ring  and the glycosidic stretching mode (–C–O–C–) [117, 120]. Typical shifts in the Raman band located at 1095 cm-1, as a function of tensile deformation for cellulose nanowhis-kers extracted from tunicates, are shown in Fig.7a . The shift plateaus at high strain due to the debonding of nanowhiskers from the matrix . The shift in the peak position of the Raman band located at 1095 cm-1, before debonding occurs, was found to be highly sensitive to the application of tensile deformation, which indicates that the molecular chains of the cellulose structure are being deformed. The rate of shift of this band with respect to strain has been related to the modulus of the whiskers. By assuming that the whiskers have a uniform stress micro-structure, it is possible to show, using an analysis by Krenchel  for a 2D random in-plane distribution of reinforcing elements, that they have a modulus of 143 GPa . A recent AFM bending experiment on single tunicate whiskers has conﬁrmed this value . Similar band shifts have been obtained for cellulose whiskers produced by acid hydrolysis of cotton, as shown in Fig.7b . Using the same analysis as used for the tunicate whiskers, moduli of 57 GPa (2D networks) and 105 GPa (3D
(a) 0 0.5 1 1.5 2 0 0.2 0.4 0.6 0.8 1 1st cycle 2nd cycle 3rd cycle ) a P M( s s ert S Strain (mm/mm) 0% (b) 0 0.5 1 1.5 2 0 0.2 0.4 0.6 0.8 1 1st cycle 2nd cycle 3rd cycle 4th cycle ) a P M( s s ert S Strain (mm/mm) 1%
Fig. 6 Thermo cycling (shape memory behaviour) of a neat SPU
(commercial) and b SPU containing 1 wt% nanocellulose .
Reproduction of image from  with permission from Wiley
networks) were obtained. These values are signiﬁcantly lower than for tunicate whiskers, which may be an indi-cation of a lower crystallinity for these nanowhiskers, possibly induced by the chemical processing route. This low value for the modulus may also arise due to the smaller aspect ratio of cellulose nanowhiskers produced by acid hydrolysis compared to tunicate whiskers, and hence an inferior stress-transfer efﬁciency.
BC nanoﬁbrils, as already discussed in the section ‘‘An overview of cellulose whisker and nanoﬁbre properties (Grenoble Institute of Technology (INPG), International School of Paper, Grenoble, France)’’, have a completely different morphology to the nanowhisker form. The nano-ﬁbrils of this form of cellulose generally form a network structure, rather like that seen in paper. The modulus of BC nanoﬁbrils has been previously measured using an AFM cantilever method, yielding a value of 78 GPa . Figure7c shows a shift recorded in the position of the 1095 cm-1band as a function of strain applied to a ﬁbrous network of BC ﬁbrils . After conﬁrming that the BC samples comprised a random 2D network of ﬁbres, it was possible to show that the modulus of an individual ﬁbril was 114 GPa . This value, although higher than the one obtained by the AFM method, is lower than the crystal modulus of cellulose (*138 GPa)  and tunicate cel-lulose whiskers. The reason for this lower value was thought to be because BC has a lower crystallinity (about 80%) than tunicate cellulose nanowhiskers .
Exploiting hydrogen bonding for the processing of cellulose nanocomposites (Case Western Reserve University, Cleveland, USA)
Jeff Capadona, Stuart Rowan and Christoph Weder at Case Western University, USA, have been investigating the ability to switch hydrogen bonding in cellulose nanocom-posites, to render them ﬂexible when immersed in water.
Owing to their strongly interacting surface hydroxyl groups, cellulose nanowhiskers have a signiﬁcant tendency for self-association . This is, in principle, a very desirable feature for the formation of load-bearing perco-lating architectures within a host polymer matrix: the spectacular reinforcement observed for polymer/cellulose nanowhisker nanocomposites can be attributed to the for-mation of rigid nanowhisker networks in which stress transfer is facilitated by hydrogen-bonding among the nanowhiskers . However, these same nanowhisker– nanowhisker interactions can also cause nanowhisker aggregation during the nanocomposite fabrication; this, of course, limits the extent of mechanical reinforcement [124,125]. Good dispersion during processing is achieved when nanowhisker self-interactions are ‘‘switched off’’ by
(a) 0.00 0.25 0.50 0.75 1.00 1.25 1.50 1.75 -2.50 -2.25 -2.00 -1.75 -1.50 -1.25 -1.00 -0.75 -0.50 -0.25 0.00 Slope = - 2.4 cm-1 /%) R2 = 0.9 m c( tfi h S d n a B n a m a R 1- ) Strain (%) (b) 0.0 0.2 0.4 0.6 0.8 1.0 1096.9 1097.0 1097.1 1097.2 1097.3 1097.4 1097.5 1097.6 1097.7 Load 1 Unload 1 Load 2 m c( r e b m u n e v a W n a m a R 1- )
Beam Surface Strain (%) Gradient = 0.87 cm-1 %-1 R2 = 0.9 0.0 0.5 1.0 1.5 2.0 2.5 -4.0 -3.5 -3.0 -2.5 -2.0 -1.5 -1.0 -0.5 0.0 0.5 (c) Sample 1 Sample 2 Gradient = -1,77 cm-1 %-1 R2 = 0.9 m c( tfi h S d n a B n a m a R 1- ) Strain (%)
Fig. 7 Shifts in the band positions for the 1095 cm-1Raman peak
from a tunicate cellulose whiskers embedded in epoxy resin and
deformed under 4-point bending in tension, b acid hydrolysed
cellulose whiskers embedded in epoxy resin and deformed under 4-point bending in tension (samples were loaded and unloaded for 1
cycle) and ctwo ﬁbrous networks of bacterial cellulose deformed
independently in tension. Reproduction of imagea from  with
permission from American Chemical Society (American Chemical
Society 2005), b from  with permission from the American
Physical Society (American Physical Society 2008) andcfrom 
with permission from Springer (Springer 2008)
competitive binding with a hydrogen-bond-forming sol-vent. Since water disperses most types of cellulose nano-whiskers well, the mixing of aqueous polymer solutions or emulsions with cellulose nanowhisker suspensions and subsequent ﬁlm casting has for a long time been the primary method to process polymer/nanowhisker nanocomposites . Furthermore, several ‘‘solubilizing schemes’’ have been explored to improve nanowhisker dispersibility in organic media, including the use of surfactants [125,126], silylation , grafting of PEO  or maleated polypro-pylene  and acylation . However, these surface modiﬁcations usually also reduce the interactions among the nanowhiskers and thereby the macroscopic mechanical properties of the corresponding nanocomposites. Turbak and co-workers have shown that stable suspensions of tunicate nanowhiskers with negatively charged sulfate groups, commonly produced by hydrolysis of the native cellulose with sulfuric acid [43,123,129], can also be pro-duced in dimethylsulfoxide (DMSO) ,N,N-dimethyl formamide (DMF) [85,86], N-methyl pyrrolidine (NMP) , formic acid  and m-cresol  for example by lyophilization of aqueous whisker dispersions and re-dis-persion of the resulting aerogel in the organic solvent . Gray has produced similar cellulose nanowhisker disper-sions in polar organic solvents using whiskers obtained from cotton . Cellulose nanowhiskers without surface charges [132,133], prepared by hydrolysis with HCl, do not disperse as well in aprotic solvents (DMSO, DMF, NMP); however, formic acid andm-cresol have been shown to also disperse non-charged nanowhiskers properly .
The ability to break hydrogen bonds and disperse cellu-lose nanowhiskers in hydrogen-bond-forming organic sol-vents opens the door for the fabrication of nanocomposites with a broad range of polymer matrices. For example, Weder and co-workers  reported nanocomposites derived from tunicate nanowhiskers and (semi)conducting p -con-jugated polymers, including doped polyaniline (PANI) and a poly(p-phenylene ethenylene) (PPE) derivative with qua-ternary ammonium side chains. These materials were solu-tion-cast from formic acid. Measurements of electrical conductivity, photoluminescence, and mechanical proper-ties reveal that the nanocomposites synergistically combine the electronic characteristics of the conjugated polymers with the outstanding mechanical characteristics of the cel-lulose scaffold. Rowan and Weder reported percolating nanocomposites with polystyrene or an ethyleneoxide/epi-chlorohydrin copolymer (EO-EPI) matrix and systemati-cally investigated such materials prepared with either tunicate or cotton nanowhiskers . In the rubbery regime of these materials, which were prepared by solution-casting from DMF, the shear moduli (G0) increased by over two orders of magnitude at a nanowhisker content of*20% v/v (Fig.8). This spectacular reinforcement is related to the
formation of a percolating nanoﬁbre network in which stress transfer is facilitated by hydrogen-bonding between the nanowhiskers. The mechanical properties can be predicted by a percolation model, which expressesG0cas [136,137]
G0c¼ð12wþwXrÞG 0 sG0rþ ð1XrÞwG0r2 ð1XrÞG0rþðXrwÞG0s ð3Þ with w¼Xr XrXc 1Xc 0:4 ð4Þ whereXris the volume fraction of the rigid (r,
nanowhis-ker) component,G0sandG0rare the shear moduli of the neat soft (s, polymer) and rigid constituents, and w is the vol-ume fraction of nanowhiskers. Figure8 shows that Eq.3 matches excellently with the experimentally determinedG0c values of EO-EPI nanocomposites comprising nanowhis-kers isolated from tunicates and cotton .
To produce cellulose nanocomposites with hydrophobic polymers, Weder and Rowan introduced a template approach to nanocomposite fabrication . The process is based on the formation of a three-dimensional template scaffold of well-individualized nanowhiskers, which is subsequently ﬁlled with a polymer of choice (Fig.9a). The ﬁrst step is the formation of a nanoﬁbre template through a sol/gel process. For cellulose nanowhiskers this involves the formation of an aqueous nanowhisker dispersion, which is converted into a gel through solvent-exchange with a
0.0 0.1 0.2 0.3 0.4 0.5 106 107 108 109 ' G c ) a P(
Volume Fraction of Whiskers
Fig. 8 Shear moduli G0 of cellulose whisker nanocomposites with EO-EPI as a function of composition. The nanocomposites were
fabricated by either solution casting (open symbols) or the template
approach (ﬁlled symbols) and shear moduli G0 were determined by
DMTA at 25C. Data are for nanocomposites comprising cellulose
whiskers isolated from tunicate whiskers (circles), cotton (squares)
and microcrystalline cellulose (triangles), respectively. Solid lines
represent predictions by the percolation model (Eq.3). Reproduction
of image with permission from AAAS (AAAS 2008)
water-miscible solvent, for example acetone, that ‘‘turns’’ the hydrogen bonding between the nanowhiskers back on. That is to say replacing the water with a weaker hydrogen bonding solvent (e.g. acetone) results in the reestablish-ment of hydrogen bonding between the whiskers. This nanoﬁbre template, which displays a percolating network structure (Fig.8b), is then ﬁlled with a matrix polymer by immersing the gel into a polymer solution, in a solvent that does not disperse the nanowhiskers, and subsequent drying and shaping. Weder and Rowan demonstrated that this technique, which is somewhat different from other recently developed ‘‘impregnation schemes’’ [32,93], is applicable to cellulose nanowhiskers isolated from tunicates, cotton, MCC and other nanoﬁbres, such as carbon nanotubes [135, 138]. To evaluate the template approach, cellulose nano-whisker nanocomposites with EO-EPI were studied in detail (Fig.8). Gratifyingly, the materials prepared by the template approach show identical mechanical properties to materials prepared by solution casting from DMF, indica-tive of the formation of percolating networks. It was pre-viously difﬁcult to incorporate cellulose nanowhiskers into non-polar polymers such as polypropylene or polybutadi-ene without surface modiﬁcation or surfactants. Thus, probably the most important feature of the template approach is its capability to access percolating nanocom-posites of otherwise immiscible components. This was demonstrated for polybutadiene/tunicate nanowhisker nanocomposites, which exhibit the mechanical properties predicted by the percolation model .
Recognizing that switching the interactions among nanowhiskers in a solid nanocomposite through an external stimulus could be a way to create a new type of mechan-ically adaptive material, Weder and Rowan took the con-cept of controlling nanowhisker–nanowhisker interactions one step further and introduced a new family of morphing materials, in which a chemical stimulus causes a signiﬁcant and reversible stiffness change [139,140]. The material’s design mimics the structural concepts at play in the dermis of sea cucumbers (Fig.10) . These creatures have the fascinating ability to rapidly and reversibly alter the stiff-ness of their skin when threatened. This dynamic mechanical behaviour is achieved through a nanocompos-ite archnanocompos-itecture, in which rigid, high-aspect-ratio collagen ﬁbrils reinforce a viscoelastic matrix (Fig.10). The stiff-ness of the tissue is regulated by controlling the ﬁbrillar interactions (through either non-covalent [141, 142] or covalent  bonds) and therewith the stress transfer, among adjacent collagen ﬁbrils by locally secreted pro-teins. Rowan and Weder prepared and studied chemo-responsive materials, which mimic this architecture and whose morphing mechanical characteristics are very simi-lar to those of the biological model [144, 145]. For example, they demonstrated that nanocomposites based on a rubbery poly(ethylene oxide) copolymer and a percolat-ing network of tunicate nanowhiskers can exhibit a reversible, 40-fold modulus reduction upon exposure to a chemical regulator that switches off the hydrogen bonds among the nanoﬁbres. This can be done through the
Fig. 9 a Schematic of the template approach to well-dispersed
polymer/cellulose whisker nanocomposites.iA non-solvent is added
to an aqueous whisker dispersion in the absence of any polymer.
iiSolvent exchange promotes the self-assembly of a nanoﬁbre gel.
iii The gelled nanoﬁbre scaffold is imbibed with a polymer by
immersion in a polymer solution, before the nanocomposite is dried
(iv) and compacted (v).bScanning electron microscopy image of a
cellulose whisker aerogel, prepared by supercritical extraction of a
whisker acetone gel (Fig.2a,ii) (scale bar=200 nm). Reproduction
of imagesaandbfrom  with permission from Nature Publishing
Group (Nature Publishing Group 2007)
addition or removal of water, which acts as a chemical regulator that changes the hydrogen bonding between the whiskers within the polymer matrix, and at the same time presumably also impacts the whisker/matrix interactions. True to the intended design, the uptake of a small amount of water causes a dramatic modulus reduction (e.g. from 800 to 20 MPa for a composite comprising 19 vol% nanowhiskers); the original stiffness is restored when the composites are dried. Control experiments and analyses using mechanical models support the conclusion that the stiffness change is due to the designed mechanism of altered nanowhisker–nanowhisker interactions, rather than alternative effects such as plasticization of the matrix. Polymerisation from the surface of cellulose whiskers (University of Nottingham, UK)
Polymers can be grown from cellulose nanowhiskers directly using the surface hydroxyl groups as initiating sites, or the surface can be modiﬁed to introduce different initiator sites needed for controlled polymerisation tech-niques such as atom transfer radical polymerisation (ATRP) or reverse addition fragmentation radical poly-merisation (RAFT). Wim Thielemans at the University of Nottingham is currently working on the surface modiﬁca-tion of cellulose nanowhiskers and has recently reported on this approach, as have some other authors.
Surface initiated polymerisation techniques have been used extensively to graft polymers from the surface of macroscopic cellulose ﬁbres [146–154]. Extending these
techniques to cellulose nanowhiskers is a logical step. Indeed, surface initiated polymerisation from the surface of cellulose nanowhiskers is currently receiving a large amount of attention and numerous presentations at con-ferences have been given [155–159]. However, to date, only four publications have appeared in the literature: Habibi et al.  reported the ring opening polymerisation of e-caprolactone using the surface hydroxyl groups as initiator sites, while both Yi et al.  and Morandi et al.  reported the grafting of polystyrene using surface initiated ATRP after grafting of an isobutyryl bromide moiety to the surface of the nanowhiskers to introduce the necessary initiator sites. Xu et al.  reported on the grafting of 6-[4-(4-methoxyphenylazo) phenoxy] hexyl-methacrylate (MMAZO) from the surface of cellulose nanocrystals using ATRP after similarly grafting an iso-butyryl bromide moiety to the surface of the nanowhiskers to introduce the necessary initiator sites. Simpliﬁed reac-tion schemes are given in Fig.11.
Grafting of poly(e-caprolactone) (PCL) from the surface of ramie cellulose nanowhiskers was performed in toluene using stannous octoate (Sn(Oct)2) as the catalyst . The authors reported a ﬁnal PCL content of 85 wt% in the modiﬁed nanowhiskers. However, as the modiﬁed nano-whiskers were not extracted but puriﬁed by a solubilisation– centrifugation sequence, ‘‘contamination’’ of the modiﬁed nanowhiskers by physically absorbed polymer chains could not be excluded. The PCL-grafted cellulose nanowhiskers were subsequently shown to increase the mechanical prop-erties of PCL-cellulose nanowhisker composites more than unmodiﬁed cellulose nanowhiskers, indicating great potential in nanocomposite reinforcement applications.
Surface initiated ATRP from the surface of cellulose nanowhiskers requires a two-step reaction: grafting of the initiator bearing a C–Br or C–Cl bond followed by polymerisation initiated by the addition of vinyl mono-mers and the catalyst Cu(I)Br (or Cu(I)Cl if using a C–Cl terminated initiator). An equilibrium between Cu(I)Br and Cu(II)Br2 (or between Cu(I)Cl and Cu(II)Cl2), the latter
formed by extraction of bromide (or chloride) from the initiator giving rise to a radical, results in controlled polymer chain growth. For surface-initiated polymerisa-tion, a dissolved sacriﬁcial initiator is sometimes used, in addition to the surface initiator groups. The use of a sacriﬁcial initiator allows the graft length to be tailored by changing the initial ratio [monomer]/[sacriﬁcial initiator] and the ﬁnal conversion (given that the amount of initi-ating sites on the nanowhiskers is negligible compared to the amount of sacriﬁcial initiator) . In addition, the non-grafted polymer chains formed through polymerisa-tion from the sacriﬁcial initiator allows for direct deter-mination of the grown polymer using standard polymer characterisation techniques to verify whether controlled
Fig. 10 a Pictures of a sea cucumber in soft and stiff state and
bschematic of the switching mechanism in this biological model and
the proposed biomimetic nanocomposites. The stress transfer among rigid, percolating nanoﬁbres, and therewith the overall stiffness of the
material, is controlled by a stimulus. Reproduction of imagesaandb
from  with permission from AAAS (AAAS 2008)
polymerisation conditions were obtained. Yi et al.  ﬁrst grafted 2-bromoisobutyryl bromide to cotton nano-whiskers, followed by styrene polymerisation without the use of a sacriﬁcial initiator. The ﬁnal polystyrene content on the nanowhiskers, puriﬁed through soxhlet extraction, was determined to be 64 wt%. The grafted polymer, removed from the surface through acid hydrolysis of the ester linkage of the initiator, was found to exhibit a rel-atively low polydispersity (PDI=1.21), showing good control of the polymerisation reaction. Through an investigation of the liquid crystalline phases of solutions of polystyrene-cellulose nanowhiskers, it was proved that the chiral nematic ordering of the cellulose nanowhiskers in solution is due to their shape, and not to the chiral nature of their surface. The same group also reported on successful grafting of poly(MMAZO) using ATRP with-out sacriﬁcial initiator to the surface of the nanowhiskers derived from the acid hydrolysis of ﬁlter paper after
derivatisation using 2-bromoisobutyryl bromide . Grafting was conﬁrmed by FTIR spectroscopy, TGA and DSC, and the grafting percentage was determined to be around 75% based on DSC data. However, no indication of the grafted chain lengths or control over the poly-merisation was reported. The grafted nanowhiskers were subsequently tested for their liquid crystalline behaviour as a solution in chlorobenzene. A lyotropic nematic phase was seen to appear, with turbidity observed at room temperature for concentrations above 5.1 wt%. Morandi et al.  ﬁrst studied various reaction conditions for the grafting of the initiator, 2-bromoisobutyryl bromide, to the surface of nanowhiskers, followed by a series of polymerisations resulting in polystyrene brushes with different graft lengths. By controlling the grafting density of the initiator they were able to control the grafting density of the ﬁnal polymer chains, while control over the polymerisation allowed them to control the length of the
OH OH OH OH O O (a) O O O H O O O H O O O H O O O H n m p q O O O H OH OH O O O H OH O O Br p n O O O H OH OH n O O O H OH O p O Br O O O H OH OH x OH OH OH OH OH Br Br Br Br Br m (b)
Fig. 11 Reaction scheme for the surface initiated polymerisation
from the surface of cellulose nanowhiskers a by ring-opening
polymerisation ofe-caprolactone, initiated from the surface hydroxyl
groups and b by ATRP through grafting of 2-bromoisobutyryl
bromide to introduce initiator sites followed by the controlled polymerisation of styrene. The grafted PCL chains are shown to have different length due to the uncontrolled nature of ring-opening polymerisation
polymer chains. A maximum surface modiﬁcation with initiator up to 70% was achieved, as well as a polystyrene content up to 22 wt%. The control over the polymer chain length and grafting density is important when the surface properties need to be speciﬁcally tailored. They subse-quently used polystyrene-grafted nanowhiskers to absorb 1,2,4-trichlorobenzene, a persistent organic pollutant, from water, opening up an interesting new application of surface modiﬁed cellulose nanowhiskers.
Analysis of dispersion of cellulose nanoﬁbres and TEMPO oxidation to induce this dispersion (Virginia Tech, USA)
One of the main challenges in the use of cellulose nano-whiskers for polymer reinforcement is achieving a uniform distribution in a matrix material. Analysis of the nano-whisker distribution in cellulose nanocomposites by transmission electron microscopy is hampered by the lim-ited contrast between the organic nanowhiskers and the organic matrix. Maren Roman at the Department of Wood Science and Forest Products, Virginia Tech, has developed a method for ﬂuorescent labelling of cellulose nanowhis-kers , potentially enabling the use of ﬂuorescence or laser scanning microscopy to analyze particle distribution in cellulose nanocomposites, as has recently been applied to clay nanocomposites [162,163].
Labelling was achieved via a three-step reaction (Fig.12) involving activation of the surface hydroxyl groups with epichlorohydrin followed by opening of the oxirane ring with ammonium hydroxide. The thus aminated crystal surface was then reacted with ﬂuorescein-50 -iso-thiocyanate (FITC) resulting in a label density of one FITC moiety per 27 nm2. The FITC-labelled cellulose nano-whiskers showed pH-sensitive absorbance in the blue and blue-green transition regions of light, resulting in a yellow appearance (Fig.12). The ﬂuorescence emission maximum of FITC occurs at 518 nm.
When analyzing particle dispersions in nanocomposites by ﬂuorescence microscopy [162, 163], the degree of particle agglomeration is deduced from the homogeneity of ﬂuorescence intensity across the specimen. Agglomerates are discernible by their higher local ﬂuorescence intensity. Laser scanning microscopy with its ability to produce a series of thin (0.1–1.5 lm) optical sections of the ﬂuores-cent specimen, which can then be stacked to produce a 3D representation, offers the possibility to analyse the disper-sion of ﬂuorescent particles in nanocomposites in thex-,y-, and z-direction. Thus, ﬂuorescent labelling of cellulose nanowhiskers in combination with ﬂuorescence or laser scanning microscopy may become a valuable tool in the optimization of processing conditions for minimal agglomeration in cellulose nanocomposites.
Adequate dispersion and distribution of ﬁbre reinforce-ment leads to optimum performance of the composite. The mechanical properties are also dictated by the length of the particle and more importantly the aspect ratio of the nanoﬁbre. To this end, great effort has gone into describing the length and diameter of acid hydrolyzed cellulose nanowhiskers. Atomic force microscopy  and trans-mission electron microscopy  studies have quantita-tively revealed average length and diameter of cellulose nanowhiskers. From these studies, nanowhiskers from wood have average lengths reported in the range between 105 and 150 nm and diameters 4.9–12 nm. Aspect ratios of the nanowhiskers are between 10 and 30. Other nanoscale celluloses like MFC maintain the length of the nanoﬁbril providing higher aspect ratios. MFC is derived from unraveling the microﬁbril structure of the cell wall using severe mechanical treatment [166,167]. This material has a unique mesh containing tens of nanometre diameter ﬁbrils appearing to have micrometer lengths.
Since the original studies in the 1980s, MFC was pro-duced with pretreatment stages that lower the energy requirement by loosening the hydrogen bonds amongst nanoﬁbrils with enzyme and chemical treatments
Fig. 12 Reaction scheme for the labelling of cellulose nanowhiskers with
ﬂuorescein-50-isothiocyanate and image
showing aqueous suspensions of
(A) cellulose nanowhiskers (0.8
wt%) and (B) FITC-labelled
cellulose nanowhiskers (0.5 wt%). Reproduction of images
aandbfrom  with
permission from American
Chemical Society (American
Chemical Society 2007)
[168, 169]. Recently, renewed interest in this material, which has dimensions of carbon nanotubes, has led to the development of low energy methods for isolation by such equipment as a blender or even a magnetic stir plate [170, 171]. Isogai and co-workers  showed that after cel-lulose pulps are oxidized in a heterogeneous suspension with 2,2,6,6 tetramethyl-1-piperidinyloxy (TEMPO) as a catalyst, the accessible primary hydroxyls on the surface of the microﬁbrils become modiﬁed with anionic carboxylate groups. As a result, the nanoﬁbrils within the ﬁbres can become unwound by mechanical agitation with repulsive forces between ionized carboxylates overwhelming the myriad of hydrogen bonds holding the nanoﬁbrils together. Solutions of nanoﬁbrils (3–5 nm diameter) are directly produced from the TEMPO-mediated oxidized pulp using mechanical agitation from a blender .
Scott Renneckar of Virginia Tech has a research pro-gram focussed on the nanoscience of cellulose and wood-based materials. Working with Johnson et al. , they have shown that TEMPO-oxidized pulp can be isolated by sonication without blending. A novel method to compare the effect of surface area on the mechanical reinforcement potential in thermoplastic composites was reported within that study; the sonication time of the TEMPO-oxidized pulp was varied inﬂuencing the yield of the nanoﬁbrils. At 20 min of sonication, 98% of the pulp was converted into nanoﬁbrils that had a width between 3 and 5 nm, according to TEM measurements (Fig.13) . These nanoﬁbrils showed better reinforcement of hydroxypropylcellulose, relative to acid hydrolyzed nanowhiskers, and 20-pass MFC (isolated without pretreatment).
With AFM, Li and Renneckar  investigated the length and thickness of TEMPO modiﬁed wood pulp ﬁbre that underwent extensive sonication and found nanoﬁbrils with unique dimensions. After 30 min of sonication, the nanoﬁbrils had an average thickness value of 1.38 nm and
length of 580 nm. If the sonication time was increased to 4 h, the average thickness of the nanoﬁbrils decreased to 0.74 nm and length to 260 nm. Interestingly, there was no correlation between length and thickness on individual nanoﬁbrils and the average aspect ratio of these materials maintained a value around 500 . This aspect ratio is remarkable for wood-based cellulose nanoﬁbres and pro-vides insight into the better composite performance high-lighted by Johnson et al. .
Applications and new advances in cellulose nanocomposites
Reinforcing adhesives using cellulose nanoﬁbres (BOKU, Vienna, Austria)
Adhesive bonding is a routine processing step in the wood industry. Potential routes for performance improvements of wood adhesives focus very much on polymer chemistry  but currently little attention is paid to the role of ﬁllers. The example of reinforced epoxy, an adhesive typically not used in the wood industry, shows that the addition of ﬁbrous ﬁller primarily improves the toughness of an adhesive bond [177–184]. Conﬁrming results achieved in modelling studies [185, 186], a comparative study of a broad variety of wood adhesives [187–189] indicated a strong correlation between the toughness of an adhesive and the ultimate shear strength of corresponding wood adhesive bonds. Urea-formaldehyde resins (UF) are a widely used class of low-priced wood adhesives, which are well known for their pronounced brittleness and their ten-dency to develop microcracks (Fig.14) which limits their mechanical performance. The combination of low price and poor mechanical performance makes UF an ideal candidate for studying the effect of added ﬁller.
Fig. 13 Nanocellulose prepared by TEMPO-mediated
oxidation of pulp;aatomic
force microscopy height image of nanocellulose deposited on
mica,b4% concentration of
nanocellulose foam after blending oxidized pulp for 18 min
A team led by Wolfgang Gindl and Josef Keckes on nanocellulose research has been investigating the rein-forcement of adhesives. For this purpose, a 5% suspension (cellulose/water) of dissolving grade beech pulp obtained from Lenzing R&D was ﬁbrillated by 20 passes through a laboratory reﬁner and, after diluting the suspension to 0.5% cellulose content, 10 passes through an APV-Gaulin high-pressure homogeniser at a high-pressure of 450 bar. Thereafter, the suspension was vacuum-dried to increase the cellulose content to 3.2%. A higher cellulose content would have been desirable in the wood adhesive, but this was limited by the rapidly increasing viscosity of the suspension with the decreasing water content. Lap-joint shear test speci-mens according to EN 302  were prepared with beech wood using the following different adhesives:
• pure UF (W-Leim Spezial, Dynea);
• UF reinforced with untreated pulp ﬁbres (5% cellulose per unit weight cured UF);
• UF reinforced with homogenised pulp ﬁbres (5% cellulose per unit weight cured UF);
and tested to failure in a universal testing machine at a speed of 1.66910-5 m s-1. The overall deformation in the overlapping region of the EN 302 specimens was recorded by means of a Zwick Macrosense clip-on deformation sensor.
The results of the mechanical tests (9 specimens each) are shown in Fig.15. With a shear strength of 10.3±0.9 MPa, the UF used in the present study is well within the range of bond strengths observed for a variety of wood adhesives in a previous study. The addition of 5% untreated pulp ﬁbres had no signiﬁcant effect on the shear strength, which was 9.9±0.8 MPa. In strong contrast, the addition of
5% reﬁner-treated and high-pressure homogenised cellulose resulted in a signiﬁcant increase of shear strength to a value of 13.8±1.4 MPa. The stress–strain curves shown in Fig.15indicate a signiﬁcantly higher deformation at failure for the specimens reinforced with homogenised pulp ﬁbres, suggesting that the UF adhesive was possibly toughened by the addition of ﬁbrillated cellulose. This assumption is supported by the fact that cracks, which are frequent in conventional UF bond lines (Fig.14), were not found when cellulose-reinforced UF was used.
The value of 13.8 MPa for the shear strength measured for cellulose-reinforced UF adhesive bonds is higher than the average shear strength of 10 MPa observed for struc-tural adhesives such as phenol–resorcinol–formaldehyde, melamine–urea–formaldehyde, and one-component poly-urethane . This indicates that the addition of ﬁbril-lated cellulose to UF signiﬁcantly improves the mechanical performance of wood adhesive bonds, thus opening up new ﬁelds of application for UF, which is currently used only in the non-structural ﬁeld.
Optically transparent cellulose nanocomposites for electronic displays (RISH, Kyoto University, Kyoto, Japan)
Flexibility is an essential characteristic not only for future electronic devices such as displays and solar cells, but also as materials suitable for roll-to-roll production processes. Roll-to-roll processing enables the continuous deposition of functional materials such as metal wiring, transparent conductive ﬁlms and gas barrier ﬁlms on a roll of optically transparent ﬂexible plastics, allowing a simple and inex-pensive processing suitable for the manufacture of ﬂexible electronic devices. Most plastics however have a large
0 3 6 9 12 15 0.00 0.05 0.10 0.15 0.20 0.25 Nominal deformation ) a P M( s s ert s r a e h S UF+Homogenised pulp UF+Pulp UF
Fig. 15 Shear stress of different lap-joint specimens plotted over deformation (the deformation is only nominal because it comprises axial and shear contributions from both the wood and the adhesive)
Fig. 14 Light microscope image of beech wood bonded with urea formaldehyde. Vertical cracks in the cured urea formaldehyde bond line are a typical result of the brittleness of this frequently used wood adhesive